Sulfur-Asphalt Site Construction Trial in Kuwait
Salah E. Zoorob and Suad K. Al-Bahar
Construction & Building Materials Program, Energy & Building Research Centre, Kuwait Institute for Scientific
Research, Kuwait City, Kuwait
Emails: firstname.lastname@example.org, email@example.com
Abstract—A full scale trial into the use of sulfur-extended
hot mix asphalt was carried out on a full depth 2 lane access
road South of Kuwait City in June 2015. The road is
composed of wearing, binder and base course hot mix
asphalt layers all in compliance with Ministry of Public
Works mix gradation specifications. Four binder types were
assessed; 60/70pen grade Kuwaiti bitumen, 2% EVA
polymer modified binder, 60/70pen modified with locally
produced sulfur and 60/70pen modified with Shell Thiopave
pellets. The trial road was divided into six longitudinal
sections to facilitate direct comparison of the performance
of the various binders types. Full depth cores were extracted
for testing from each of the six sections soon after the
completion of construction and after 1 year of opening to
traffic. The paper includes details of the site layout,
granular subbase and asphalt compaction, variation in
asphalt mix density and voids, indirect tensile stiffness
determinations, moisture conditioning and wheel tracking
tests. Overall, both sulfur extended asphalt mixes performed
better than the conventional 60/70pen mix, in particular
with respect to stiffness and creep performance.
Significantly, compared to the 60/70pen mix, the sulfur-
extended mixes ageing with time could not be explained
entirely by environmental exposure related oxidative
Index Terms—hot mix asphalt, sulfur-extender, thiopave,
full scale site construction
I. AN OVERVIEW OF SULFUR-EXTENDED HOT MIX
A. Background to Sulfur-Extended Asphalt
In the early 1970s, due to concern over asphalt cement
(bitumen) supply issues and an anticipated
overabundance of elemental sulfur, several organizations
in the U.S. and Canada, began to evaluate the potential
for sulfur to substitute for bitumen as binder extender,
this became known as Sulfur Extended Asphalt.
In the late 1980s, a sharp rise in the price of sulfur in
addition to the fact that the use of hot liquid sulfur during
production generated a significant amount of noxious
fumes brought its use in road paving to an end. However,
more recent rises in bitumen prices coupled with the
production of low sulfur fuels has once again made sulfur
a marketable product in the asphalt industry.
To overcome the problems with hot liquid sulfur used
in bituminous mixes, Sulfur Extended Asphalt Modifier
in solid pellet form (patented process) was developed and
Manuscript received January 5, 2017; revised May 5, 2017.
is currently being marketed as an additive for hot mix
asphalt under the brand name Shell Thiopave
Thiopave pellets are in a solid, non-sticky, non-melting
form at ambient temperatures, which eases handling,
storage and transportation. The pellets have melting point
in the range 93 to 104°C, which has been specifically
designed to melt when in contact with Hot Mix Asphalt
(HMA). Thiopave is intended to act both as a bitumen
extender and as an asphalt mixture modifier.
The key to the composition of Thiopave is that liquid
sulfur is plasticized by the addition of carbon black (0.4
to 0.8%) and the plasticized sulfur is further treated with
amyl acetate (0.2 to 0.4%) to produce an even more
manageable plasticized sulfur additive. Amyl acetate
helps to reduce unwanted odours from the product and
thereby improve its overall handling .
B. Manufacturing and Laying Sulfur Extended Asphalts
Sulfur may be used in asphalt mixes made with
conventional bitumen in weight ratios from 20%/80% to
50%/50% Sulfur/Bitumen. Stiffness and Marshall
stability are expected to increase with increased amounts
of sulfur . Once a Sulfur/Bitumen ratio is selected, the
equivalent volume replacement of binder (by % weight)
can be determined. Since sulfur is about twice as dense as
bitumen, a given weight of sulfur has about half the
volume of the same weight of bitumen .
The sulfur pellets at ambient temperature are added to
the pre-heated aggregate and bitumen during the HMA
production process. The addition can be achieved via a
feeder in an asphalt batch plant or via the reclaimed
asphalt collar in a continuous mixing plant.
For health and safety reasons, the manufactures stress
that when incorporating sulfur additive, the asphalt mix
discharge temperatures must be carefully controlled to
never exceed the recommended range 135-146°C. At this
temperature, the pellets melt quickly and the shear
conditions in the mixer are high enough to disperse the
sulfur into the HMA mix in a very short time that is
compatible with asphalt mix production.
It is recommended that Sulfur-Extended HMA storage
time be kept to a minimum in order to minimize mix odor
and fume emissions at the paving site. Delayed delivery
trucks arriving at the paving site with Sulfur Extended
HMA below approximately 115 °C shall be rejected .
C. Dissolution and Reactions between Sulfur & Bitumen
When sufur and bitumen are heated and combined,
three distinct types of reactions may occur , :
International Journal of Structural and Civil Engineering Research Vol. 6, No. 3, August 2017
© 2017 Int. J. Struct. Civ. Eng. Res.
a) The sulfur can react chemically with the bitumen
and result in dehydrogenation (sulfurization through
attack of the double bonds in the bitumen). This becomes
important at temperatures above about 152°C.
Dehydrogenation occurs and hydrogen sulphide gas is
formed, which results in significant changes in the
rheological properties of the bitumen.
b) The sulfur can be dissolved in the bitumen, in a
different mechanism from the chemical dehydrogenation
c) Sulfur in the crystalline form can remain in
suspension in the bitumen.
In one study, Differential Scanning Calorimetry
analysis of Sulfur-bitumen blends containing 35% sulfur
(by mass of bitumen) showed that 70% of the sulfur in
the blend remained in immiscible crystalline form, with
the remainder 30% being amorphous. Visual monitoring
of the same bitumen/sulfur blends stored at room
temperature for up to 1 month showed the emergence of a
solid phase segregated on the surface of the samples
which was also confirmed to be crystalline sulfur .
The larger the amount of added sulfur to a bitumen, the
larger the amount of sulfur that ends up not in solution
and hence existing in a crystalline state. The result is
large amounts of crystalline sulfur existing in the paving
mixture generally as ‘needle-like’ structures most
prevalent in the mix voids. The driving force for
nucleation and growth of the sulfur needles is believed to
be provided by the solubility differences at mixing and
ambient temperatures .
D. General Findings from Full Scale Trials
As early as 1989, a large full scale investigation was
conducted by the California Department of
Transportation to determine whether the incorporation of
sulfur with a soft grade of bitumen could change the
temperature-viscosity relationship of the resulting binder,
thereby making it more useful in cold and hot climates
. The two trial sections (a hot and a cold climate test
sections) utilized the same sulfur/bitumen blends, i.e.
20% and 40% sulfur by weight of total binder, and each
project used the same blending AR 2000 bitumen (i.e.
RTFOT Residue with viscosity of 2000 Poise at 60°C).
Overall, based on the findings of this full scale study,
sulfur-extended binders were a viable alternative to
conventional bitumens. Results of physical tests (Hveem
system) on compacted briquettes and field cores revealed
no significant differences in stability, cohesion and
surface abrasion between sulfur-extended and
conventional asphalt mixes. The findings of this study
raised one major concern, in that it appeared that sulfur-
extended blends with over 20% sulfur by weight (e.g. at a
40%/60% sulfur/bitumen ratio) should not be utilized in
overlays in colder climate areas due to an early thermal
cracking potential. This was not an issue for the hotter
climate test section .
The U.S. Federal Highway Administration also
completed a field study in 1990 to compare the
performance of sulfur-extended asphalt pavements to
conventional asphalt control pavements. A re